| ||Format||Pages||Price|| |
|3||$46.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$46.00||  ADD TO CART|
|Standard + Redline PDF Bundle||6||$54.00||  ADD TO CART|
Significance and Use
5.1 Outdoor exposure tests at one location may not be applicable to a project site at another location. This test method evaluates geotextiles under site specific atmospheric conditions over an 18-month period. A degradation curve as per , based on strength, elongation, or modulus, or all of these, may be developed for the geotextile being evaluated.
5.2 This test method can be used for comparative testing of the degradation of geotextiles.
5.3 This test method is considered to be a performance test and as such the responsibility for its performance rests with the specifying or purchasing agency.
Note 1: The intent of this procedure is to provide the user of this test method and geotextiles a standard by which to evaluate weathering degradation in terms of site specific conditions, not in terms of incident radiation and temperature. If desired, the user may want to have the necessary measurement and recording equipment at each site to do this. However, the expense of doing so at each site may be prohibitive. Therefore, this is not a specific requirement of this test method.
1.1 This test method covers evaluating the deterioration in tensile strength and strain after outdoor exposure.
1.2 The deterioration is assessed as a reduction in strength and strain at failure from the unexposed geotextile.
1.3 The specific location of the light and weather exposure is made on the basis of a site specific decision between the parties involved.
1.4 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D4439 Terminology for Geosynthetics
D5035 Test Method for Breaking Force and Elongation of Textile Fabrics (Strip Method)
G7/G7M Practice for Atmospheric Environmental Exposure Testing of Nonmetallic Materials
G113 Terminology Relating to Natural and Artificial Weathering Tests of Nonmetallic Materials
ICS Number Code 59.080.70 (Geotextiles)
UNSPSC Code 30121702(Geotextile)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D5970 / D5970M-16, Standard Test Method for Deterioration of Geotextiles from Outdoor Exposure, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top